| ||Format||Pages||Price|| |
|4||$46.00||  ADD TO CART|
|Hardcopy (shipping and handling)||4||$46.00||  ADD TO CART|
|Standard + Redline PDF Bundle||8||$54.00||  ADD TO CART|
Significance and Use
4.1 When uniaxial force is applied to a solid, it deforms in the direction of the applied force, but also expands or contracts laterally depending on whether the force is tensile or compressive. If the solid is homogeneous and isotropic, and the material remains elastic under the action of the applied force, the lateral strain bears a constant relationship to the axial strain. This constant, called Poisson’s ratio, is an intrinsic material property just like Young’s modulus and Shear modulus.
4.2 Poisson's ratio is used for design of structures where all dimensional changes resulting from application of force need to be taken into account, and in the application of the generalized theory of elasticity to structural analysis.
4.3 In this test method, the value of Poisson's ratio is obtained from strains resulting from uniaxial stress only.
4.4 Above the proportional limit, the ratio of transverse strain to axial strain will depend on the average stress and on the stress range for which it is measured and, hence, should not be regarded as Poisson’s ratio. If this ratio is reported, nevertheless, as a value of “Poisson’s ratio” for stresses below the proportional limit, the range of stress should be reported.
4.5 Deviations from isotropy should be suspected if the Poisson’s ratio, μ, determined by the method described below differs significantly from that determined when the ratio E/G of Young’s modulus, E, to shear modulus, G, is substituted in the following equation:
where E and G must be measured with greater precision than the precision desired in the measurement of μ.
4.6 The accuracy of the determination of Poisson's ratio is usually limited by the accuracy of the transverse strain measurements because the percentage errors in these measurements are usually greater than in the axial strain measurements. Since a ratio rather than an absolute quantity is measured, it is only necessary to know accurately the relative value of the calibration factors of the extensometers. Also, in general, the values of the applied forces need not be accurately known. It is frequently expedient to make the determination of Poisson's ratio concurrently with determinations of Young's modulus and the proportional limit.
1.1 This test method covers the determination of Poisson’s ratio from tension tests of structural materials at room temperature. This test method is limited to specimens of rectangular section and to materials in which and stresses at which creep is negligible compared to the strain produced immediately upon loading.
1.2 The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.4 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E4 Practices for Force Verification of Testing Machines
E6 Terminology Relating to Methods of Mechanical Testing
E8 Test Methods for Tension Testing of Metallic Materials
E83 Practice for Verification and Classification of Extensometer Systems
E111 Test Method for Youngs Modulus, Tangent Modulus, and Chord Modulus
E177 Practice for Use of the Terms Precision and Bias in ASTM Test Methods
E1012 Practice for Verification of Testing Frame and Specimen Alignment Under Tensile and Compressive Axial Force Application
ICS Number Code 19.060 (Mechanical testing)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM E132-17, Standard Test Method for Poisson’s Ratio at Room Temperature, ASTM International, West Conshohocken, PA, 2017, www.astm.orgBack to Top